- Email: [email protected]

A shear-lag model for carbon nanotube-reinforced polymer composites X.-L. Gao b

a,*

, K. Li

b

a Department of Mechanical Engineering, Texas A&M University, 3123 TAMU, College Station, TX 77843-3123, USA Department of Mechanical Engineering—Engineering Mechanics, Michigan Technological University, 1400 Townsend Drive, Houghton, MI 49931-1295, USA

Received 2 February 2004; received in revised form 22 August 2004 Available online 13 October 2004

Abstract A shear-lag model is developed for carbon nanotube-reinforced polymer composites using a multiscale approach. The main morphological features of the nanocomposites are captured by utilizing a composite cylinder embedded with a capped nanotube as the representative volume element. The molecular structural mechanics is employed to determine the eﬀective YoungÕs modulus of the capped carbon nanotube based on its atomistic structure. The capped nanotube is equivalently represented by an eﬀective (solid) ﬁber having the same diameter and length but diﬀerent YoungÕs modulus, which is determined from that of the nanotube under an isostrain condition. The shear-lag analysis is performed in the context of linear elasticity for axisymmetric problems, and the resulting formulas are derived in closed forms. To demonstrate applications of the newly developed model, parametric studies of sample cases are conducted. The numerical results reveal that the nanotube aspect ratio is a critical controlling parameter for nanotube-reinforced composites. The predictions by the current analytical model compare favorably with the existing computational and experimental data. Ó 2004 Elsevier Ltd. All rights reserved. Keywords: Carbon nanotube; Nanocomposite; Shear-lag model; Interfacial stress transfer; Multiscale modeling; Polymer composite; Elasticity; Molecular structural mechanics

*

Corresponding author. Tel.: +1 979 845 4835; fax: +1 979 845 3081. E-mail address: [email protected] (X.-L. Gao).

0020-7683/$ - see front matter Ó 2004 Elsevier Ltd. All rights reserved. doi:10.1016/j.ijsolstr.2004.08.020

1650

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1. Introduction Carbon nanotubes have been identiﬁed as promising reinforcing materials for high-performance nanocomposites (e.g., Ajayan et al., 2000; Thostenson et al., 2001; Maruyama and Alam, 2002). To this end, however, many critical issues are yet to be resolved, one of which is the lack of accurate understanding of mechanisms of load transfer from the matrix to the nanotubes (e.g., Wagner, 2002). Eﬀorts have been made to assess the ability of stress transfer through the nanotube–matrix interface (e.g., Wagner et al., 1998; Schadler et al., 1998; Qian et al., 2000; Lordi and Yao, 2000; Liao and Li, 2001; Frankland et al., 2002, 2003; Frankland and Harik, 2003; Barber et al., 2003). These studies, being based on experimental measurements or molecular dynamics simulations, tend to be expensive and conﬁguration/material speciﬁc. The use of continuum-based models can mitigate these diﬃculties (e.g., Odegard et al., 2002; Zhang et al., 2002; Li and Chou, 2003a; Gao and Li, 2003; Pantano et al., 2004) and is, therefore, very desirable. The interfacial shear strength in polymer composites reinforced by single-walled carbon nanotubes has recently been estimated by Wagner (2002) using a modiﬁed Kelly–Tyson approach that is continuum-based and assumes uniform interfacial shear and axial normal stresses. More recently, a continuum-based computational model for interfacial stress transfer in nanotube-reinforced polymer composites has been developed by Li and Chou (2003b), which employs the molecular structural mechanics proposed by the same authors (Li and Chou, 2003a) to characterize the nanotube and the ﬁnite element method to model the polymer matrix. This study sheds new light on the understanding of the load transfer across the nanotube–matrix interface and provides needed guidance for the development of analytical models. The stress transfer problem for traditional ﬁber-reinforced composites has been extensively studied. The shear-lag model originally proposed by Cox (1952) provides a good estimate of the stresses in the ﬁber transferred from the matrix through the interface. However, this analytical model cannot be directly applied to characterize nanotube-reinforced composites, since it considers the load transfer across the curved interface only and regards the ﬁber ends as traction-free. In addition, some important morphological features of nanotube-reinforced composites are not incorporated in existing shear-lag models. It is known that the eﬃciency of the nanotube reinforcement depends sensitively on the morphology (including diameter, wall thickness and chirality) and distribution of the nanotubes (e.g., Thostenson and Chou, 2003). This necessitates the incorporation of atomistic structures of carbon nanotubes in developing continuum-based analytical models of shear-lag type for nanotube-reinforced composites. The objective of the current study is to develop such a shear-lag model using a representative volume element (RVE) of a concentric composite cylinder embedded with a capped carbon nanotube. The rest of the paper is organized as follows. In Section 2, the molecular structural mechanics of Li and Chou (2003a), together with the matrix method for spatial frames (e.g., Li et al., 2003), is ﬁrst employed to predict the eﬀective YoungÕs modulus of the nanotube. The capped nanotube is then replaced by an eﬀective (solid) ﬁber, whose length and diameter are kept to be the same as those of the nanotube to preserve the essential morphological features of the nanocomposite. The YoungÕs modulus of the eﬀective ﬁber is subsequently determined under an isostrain condition. This is followed by the development of the shear-lag model in Section 3 using the cylindrical RVE. In Section 4, sample numerical results are presented to demonstrate applications of the newly developed model. The paper concludes with a summary in the ﬁfth and last section.

2. Capped nanotube as an eﬀective ﬁber After numerous eﬀorts by many researchers, it has become possible to fabricate nanotube-reinforced polymer composites with well-dispersed and well-aligned nanotubes (e.g., Haggenmueller et al., 2000; Bower et al., 2000; Thostenson and Chou, 2002; Cooper et al., 2002). As a ﬁrst step toward simulating such

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1651

Fig. 1. Model nanocomposite.

Fig. 2. RVE of the model nanocomposite.

composites using continuum-based analytical approaches, consider a model composite reinforced by uniformly distributed and perfectly aligned identical nanotubes, as shown in Fig. 1. The representative volume element (RVE) of the composite is sketched in Fig. 2, where the nanotube with two end caps is regarded as perfectly bonded to the matrix and located at the center of the RVE, with both the matrix and the nanotube phases being isotropic. The cylindrical RVE of this type has been adopted earlier by Li and Chou (2003b), but in their model the nanotube is assumed to be uncapped. The shear-lag model to be developed will be based on the RVE shown in Fig. 2. The development of this continuum model requires that the structurally discrete nanotube be replaced by a continuum phase. To this end, the capped nanotube embedded in the matrix will ﬁrst be represented as an eﬀective (solid) ﬁber, whose YoungÕs modulus is determinable from that of the nanotube. The latter will be predicted using the molecular structural mechanics approach advanced by Li and Chou (2003a), which incorporates the atomistic structure of the nanotube and is based on the equivalence of the strain energy and the molecular potential energy. A fairly large number of studies have been conducted to predict elastic properties of carbon nanotubes without caps. In contrast, very limited attention has been paid to capped nanotubes, although numerous experiments indicate that carbon nanotubes are usually closed at both ends (Harris, 1999). This is partially due to the complexity associated with nanotube capping. For example, it has been shown by Fujita et al. (1992) that only nanotubes that are larger than the archetypal (5, 5) and (9, 0) tubes are capable of being capped, and that the number of possible caps grows signiﬁcantly with the increase of the nanotube diameter. The chirality and diameter of a nanotube can be uniquely determined by the roll-up (chiral) vector (m, n) (e.g., Saito et al., 1993; Thostenson et al., 2001), where m and n are non-negative integers representing the number of steps along the zigzag carbon bonds of the hexagonal lattice. A carbon nanotube designated by (m, n) is generally chiral, unless m = n or n = 0 to become an armchair or zigzag nanotube. A capped carbon nanotube (graphene tubule) may be formed by adding hexagons between two hemispheres cut from an icosahedral fullerene, which corresponds to a spherical Goldberg polyhedron

1652

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

(Fujita et al., 1992). Through deﬁning a chiral vector (mf, nf) for specifying an icosahedral fullerene, where mf and nf are non-negative integers, the total number of atoms for the fullerene is given by 20ðm2f þ mf nf þ n2f Þ. When mf = nf or mf nf = 0, two groups of fullerenes with the icosahedral symmetry (Ih) are obtained, i.e., the series of C 60 ; C 240 ; . . . ; C 60n2 and the series of C 20 ; C 80 ; . . . ; C 20n2 (where C20 is unaf f ble to nucleate a tubule). In other cases, the fullerenes have the I symmetry (which is a subset of Ih involving no inversion operation). The carbon nanotube that nucleates from two halves of a fullerene can be designated by (5mf, 5nf). Another group of zigzag nanotubes, i.e., (9, 0),(18, 0), . . ., (9nf, 0), can be capped by hemispheres cut from icosahedral fullerenes C 60 ; C 240 ; . . . ; C 60n2 , which correspond to the chiral vectors f (1, 1), (2, 2), . . ., (nf, nf), in a direction perpendicular to one of the three-fold axes (Saito et al., 1992). The caps for armchair nanotubes (5, 5), (10, 10), . . ., (5nf, 5nf) are obtained by bisecting the same group of fullerenes in a direction perpendicular to one of the ﬁve-fold axes (Saito et al., 1992). Halves of fullerene C60 could cap armchair nanotube (5, 5) or zigzag nanotube (9, 0), the two smallest carbon nanotubes that can be capped. Using molecular dynamics (MD) simulations, Yao and Lordi (1998) modeled capped single-walled and multi-walled carbon nanotubes with armchair chirality. By assuming that nanotubes are made of a continuum and employing HarrisonÕs tight-binding model, Glukhova et al. (2003) estimated the average YoungÕs modulus of capped zigzag carbon nanotubes. However, molecular dynamics and tight-binding methods typically involve extensive computations and, therefore, are limited to modeling systems embracing a small number of atoms and undergoing a short period of time. In contrast, the molecular structural mechanics (MSM) approach developed by Li and Chou (2003a) is computationally eﬃcient. By viewing a nanotube as a spatial frame, the covalent bonds between carbon atoms as equivalent structural beams and individual atoms as joints, they showed that a linkage between structural mechanics and molecular mechanics can be established. Then, the cross-sectional parameters of the equivalent beams (with circular cross-sections), which are required to form the elemental stiﬀness matrices for structural mechanics analysis based on the matrix method for spatial frames, can be determined from the equivalence of the corresponding steric potential energies of atomic bonds and elemental strain energies of structural beams. Therefore, the MSM approach of Li and Chou is employed here to calculate the eﬀective YoungÕs modulus of each capped single-walled carbon nanotube. The computer program developed by Li et al. (2003) for the matrix method in a more general context is used in the calculation to determine the displacements at unrestrained joints. Three capped armchair nanotubes, i.e., (5, 5), (10, 10) and (15, 15), and ﬁve capped zigzag nanotubes, i.e., (9, 0), (10, 0), (15, 0), (20, 0) and (25, 0), with diﬀerent values of axial length, are considered in the current ˚ 2, kh/2 = 63 kcal mol1 rad2 study. The force ﬁeld constants are taken to be kr/2 = 469 kcal mol1 A 1 2 and ks/2 = 20 kcal mol rad , and the initial carbon–carbon bond length to be 0.1421 nm, all as initially used in Li and Chou (2003a). Due to symmetry, only half of a nanotube needs to be modeled, as shown in Fig. 3. Also, the open end may be reviewed as a ﬁxed support with no displacement or rotation. By applying a concentrated axial force F to each of the joints on the cap, the YoungÕs modulus of the nanotube, Et, can be determined as

Fig. 3. Half of a capped nanotube: (a) armchair (b) zigzag.

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

Et ¼

bFLs ; 2patDLs

1653

ð1Þ

where a is the outer radius of the nanotube, t is the tube wall thickness [taken to be 0.34 nm, the interlayer spacing of graphite sheets, as was done in Li and Chou (2003a)], Ls is the length from the open end to the tube-cap intersection, DLs is the axial displacement of each joint at the intersection that is obtained using the matrix method mentioned above, and b is the total number of joints on the cap including those at the intersection. With the involvement of t in Eq. (1), the degree of hollowness of the nanotube is automatically accounted for in determining Et. The predicted values of YoungÕs modulus (Et) versus the aspect ratio (Lt/a) for uncapped nanotubes are presented in Figs. 4 and 5. From these two ﬁgures, one can observe that the trend of Et varying with Lt/a is similar for both the armchair and zigzag nanotubes. It is also seen that Et increases rapidly with Lt/a when Lt/a < 10, beyond which Et remains almost constant. A further inspection of these two ﬁgures indicates that Et increases monotonically with the nanotube diameter. For capped nanotubes, as shown in Figs. 6 and 7, the trend of Et varying with Lt/a is similar to that of the uncapped nanotubes. The aspect ratio Lt/a has little inﬂuence on Et for armchair nanotubes (see Fig. 6). (5,5) (10,10) (15,15)

1.06

Et (TPa)

1.04 1.02 1 0.98 0.96 0.94 0

20

L t /a

40

60

Et (TPa)

Fig. 4. YoungÕs modulus of uncapped nanotubes (armchair).

(9,0) (10,0) (15,0) (20,0) (25,0)

1.04 1.03 1.02 1.01 1 0.99 0.98

0

20

L t /a

40

60

Et (TPa)

Fig. 5. YoungÕs modulus of uncapped nanotubes (zigzag).

(15,15) (10,10) ( 5, 5)

1.041 1.04 1.039 1.038 1.037 1.036 1.035 1.034 0

20

40 L t /a

60

80

Fig. 6. YoungÕs modulus of capped nanotubes (armchair).

1654

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667 (9,0) (10,0) (15,0) (20,0) (25,0)

1.04

E t (TPa)

1.03 1.02 1.01 1 0.99 0

20

40 L t /a

60

80

Fig. 7. YoungÕs modulus of capped nanotubes (zigzag).

For zigzag nanotubes, Et increases with Lt/a when Lt/a is small, but remains almost constant when Lt/ a > 20 (see Fig. 7). The increasing rate (i.e., slope) here appears to be smaller than that of the corresponding uncapped zigzag nanotube (see Figs. 5 and 7). When Lt/a is ﬁxed, the eﬀect of the nanotube diameter 2a on Et is shown in Fig. 8. It is seen that the armchair nanotubes are stiﬀer than the zigzag nanotubes and the diﬀerence in YoungÕs modulus is reduced as 2a increases, which agrees with the earlier ﬁndings by Popov et al. (2000) based on a lattice dynamics model and Chang and Gao (2003) using molecular mechanics. From Fig. 8, one can also observe that for armchair nanotubes the capped ones are slightly stiﬀer than the uncapped ones when 2a < 1.3 nm, and that the stiﬀness diﬀerence decreases as 2a increases. For zigzag nanotubes, the diﬀerences in YoungÕs modulus of the capped and uncapped ones are negligibly small. These observations indicate that the eﬀect of capping is insigniﬁcant for suﬃciently long and large nanotubes. With the eﬀective YoungÕs modulus of the nanotube determined based on its atomistic structure, the nanotube embedded in the matrix can then be replaced by an eﬀective (solid) ﬁber having the same length and outer diameter as those of the nanotube (see Fig. 9). The latter are adopted to preserve the morphological features of the nanotube as the reinforcing phase. As a result, the elastic properties of the eﬀective ﬁber will diﬀer from those of the nanotube and need to be determined separately. Under an isostrain condition, the eﬀective YoungÕs modulus of the eﬀective ﬁber, Ef, can be readily obtained as

1.05

Et (TPa)

1.04 1.03 armchair-uncapped zigzag-uncapped armchair-capped zigzag-capped

1.02 1.01 1 0

0.5

1 1.5 2a (nm)

2

2.5

Fig. 8. YoungÕs modulus of nanotubes (Lt/a = 50).

Fig. 9. Nanotube as an eﬀective ﬁber.

f

E (TPa)

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1655

(5,5) (10,10) (15,15)

1.2 1 0.8 0.6 0.4 0.2 0 0

20

40 L t /a

60

80

f

E (TPa)

Fig. 10. YoungÕs modulus of eﬀective ﬁbers (armchair).

(9,0) (10,0) (15,0) (20,0) (25,0)

1.2 1 0.8 0.6 0.4 0.2 0 0

20

40 L t /a

60

80

Fig. 11. YoungÕs modulus of eﬀective ﬁbers (zigzag).

Table 1 Diameter and YoungÕs modulus of the eﬀective ﬁber Armchair

2a (nm)

E f (TPa)

Zigzag

2a (nm)

E f (TPa)

(5, 5) (10, 10) (15, 15)

0.6834 1.3594 2.0370

1.035 0.779 0.578

(9, 0) (10, 0) (15, 0) (20, 0) (25, 0)

0.7086 0.7866 1.1774 1.5684 1.9598

1.006 0.995 0.845 0.702 0.594

2

Ef ¼

a2 ða tÞ Et : a2

ð2Þ

In obtaining Eq. (2) use has also been made of the condition that the axial load carried by the eﬀective ﬁber, P, is the same as that by the nanotube. The isostrain approximation invoked here is consistent with the shear-lag analysis to be presented next. With both the outer radius (a) and the wall thickness (t) of the nanotube involved in Eq. (2) as two independent variables, the hollowness of the nanotube is directly incorporated in the determination of Ef. The calculated values of Ef as a function of Lt/a are shown in Figs. 10 and 11. Both ﬁgures clearly indicate that the larger the tube diameter is the lower Ef becomes, while Lt/a has negligible eﬀect on Ef. For convenience of later reference, the values of Ef for the diﬀerent nanotubes considered are also listed in Table 1. 3. Shear-lag model for the nanocomposite The classical shear-lag model originated by Cox (1952) was later elucidated by McCartney (1992) and Nairn (1997) in the context of linear elasticity. However, in their concentric cylinder models the ﬁber

1656

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667 x Lt

Lt

a

σ

o

z

σ

R

y 2L

Fig. 12. RVE for the nanocomposite.

and the matrix layer are equally long and the ﬁber ends are treated as traction-free ﬁber breaks (cracks). As a result, their models cannot be directly applied to the conﬁguration shown in Fig. 2 or Fig. 12. This necessitates the current shear-lag formulation using the theory of elasticity. Since the purpose of the shear-lag analysis is to describe the mechanisms of load transfer across the entire nanotube–matrix interface, which can be viewed as a global response, the use of continuum mechanics (elasticity) should lead to fairly accurate simulations (Liu and Chen, 2003). In fact, several elasticity-based models have been shown to be capable of accurately predicting the global properties of nanostructured materials (e.g., Lourie et al., 1998; Govindjee and Sackman, 1999; Ru, 2000; Harik, 2001, 2002; Lilleodden et al., 2003). The derivations presented here are built upon the earlier works of McCartney (1992) and Nairn (1997), and, therefore, the three major assumptions inherent in a shear-lag analysis, which are also invoked in the current formulation (see Eqs. (12), (19), (22) and (28) below), will not be discussed any further. The formulation is based on the RVE illustrated in Fig. 12, where the eﬀective ﬁber (continuum) has replaced the capped nanotube (discrete) (see Figs. 2 and 9). The governing equations for the axisymmetric problem, in a displacement formulation and in terms of the polar coordinates (r, h, z), include the equilibrium equations (in the absence of body forces): orrr osrz rrr rhh þ þ ¼ 0; or oz r

osrz orzz srz þ þ ¼ 0; or oz r

ð3a;bÞ

the geometrical equations: err ¼

ou ; or

u ehh ¼ ; r

ezz ¼

ow ; oz

crz ¼

ou ow þ ; oz or

ð4a–dÞ

and the constitutive equations: 1 ½rrr mðrhh þ rzz Þ; E 1 ezz ¼ ½rzz mðrrr þ rhh Þ; E err ¼

1 ½rhh mðrzz þ rrr Þ; E srz crz ¼ : G ehh ¼

ð5a–dÞ

In Eqs. (3a,b)–(5a–d), rrr, rhh, rzz and srz are stress components, err, ehh, ezz and crz are strain components, u and w are, respectively, the radial and axial displacement components, and E, m and G are, respectively, the YoungÕs modulus, PoissonÕs ratio and shear modulus of the material. These three sets of equations are applicable to both the eﬀective ﬁber and the matrix. The boundary conditions for this problem are given by tm jr¼R ¼ 0;

tm jz¼ L ¼ re3 ;

ð6a;bÞ

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1657

and the interfacial traction continuity conditions by tf jr¼a;Lt 6z6Lt ¼ tm jr¼a;Lt 6z6Lt ;

tf jz¼ Lt ;06r6a ¼ tm jz¼ Lt ;06r6a ;

ð7a;bÞ

where t is the traction vector, r is the axial normal stress uniformly applied on z = ± L, and the superscripts f, m denote, respectively, the eﬀective ﬁber and the matrix. The exact solution of the boundary-value problem deﬁned by Eqs. (3a,b)–(7a,b) for the current composite cylinder problem involving the two phases with ﬁnite dimensions (see Fig. 12) can hardly be obtained. In fact, no closed-form solution has been derived even for the simpler problem of a ﬁnite composite cylinder without the two pure matrix regions using elasticity (Smith and Spencer, 1970; Wu et al., 2000). Hence, an approximate solution of the shear-lag type will be sought here, which satisﬁes, exactly or on average, the governing equations in the longitudinal direction. The derivation will be done separately for the reinforced region (Lt 6 z 6 Lt) and the pure matrix regions (L 6 z 6 Lt and Lt 6 z 6 L). 3.1. Solution in the reinforced region (Lt 6 z 6 Lt ) Note that Eq. (3b), which is the equilibrium equation in the z-direction, can be integrated with respect to r from 0 to a to give, for the eﬀective ﬁber, Z a f Z a 1 orzz 1 1 o f rs ð2prÞdr ¼ 0: ð8Þ ð2prÞdr þ 2 2 pa 0 oz pa 0 r or rz The average axial normal stress over the cross-section of the eﬀective ﬁber can be deﬁned as Z a 1 rfzz ðzÞ 2 rf ðr; zÞð2prÞdr: pa 0 zz

ð9Þ

Then, Eq. (8) becomes, with the use of Eq. (9), drfzz 2 ¼ si ; a dz

ð10Þ

where si sfrz jr¼a

ð11Þ

is the interfacial shear stress (on the curved interface r = a), which is a function of z. To determine sfrz using the interfacial shear stress si, assume that orfzz ¼ f ðzÞ; oz

ð12Þ

where f(z) is a function yet to be determined. Then, using Eq. (12) in Eq. (3b) and integrating with respect to r from 0 to r will lead to 1 ð13Þ sfrz ¼ rf ðzÞ; 2 where use has been made of the fact that both sfrz and f(z) are ﬁnite at r = 0. By applying Eq. (11) to Eq. (13), f(z) and thus sfrz will then be determined as 2 f ðzÞ ¼ si ðzÞ; a

r sfrz ¼ si : a

ð14a;bÞ

In component form, Eq. (6a) becomes rm rr jr¼R ¼ 0;

sm zr jr¼R ¼ 0;

ð15a;bÞ

1658

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

and Eq. (7a) reads rfrr jr¼a;Lt 6z6Lt ¼ rm rr jr¼a;Lt 6z6Lt ;

sfzr jr¼a;Lt 6z6Lt ¼ sm zr jr¼a;Lt 6z6Lt :

ð16a;bÞ

Now integrating Eq. (3b) with respect to r from a to R yields for the matrix, with the use of Eqs. (11), (15b) and (16b), drm 2a zz ¼ 2 si ; dz R a2

ð17Þ

where rm zz ðzÞ

1 2 pðR a2 Þ

Z

R

rm zz ðr; zÞð2prÞdr

ð18Þ

a

is the average axial normal stress over the cross-section of the matrix layer. Similar to that for determining sfrz (see Eq. (12)), it is assumed that orm zz ¼ gðzÞ; oz

ð19Þ

where g(z) is a yet-unknown function. Substituting Eq. (19) into Eq. (3b) and integrating with respect to r from r to R will yield, with the help of Eq. (15b), 1 R2 m srz ¼ r gðzÞ: ð20Þ 2 r It then follows from Eqs. (20), (16b) and (11) that 2 2a a R m r si : si ðzÞ; srz ¼ 2 gðzÞ ¼ 2 R a2 R a2 r Next, assume that for both the eﬀective ﬁber and matrix, ou ow: oz or

ð21a;bÞ

ð22Þ

This leads to, using Eqs. (4d) and (5d), sfrz ¼ Gf

owf ; or

m sm rz ¼ G

owm : or

ð23a;bÞ

Combining Eqs. (21b) and (23b) and integrating with respect to r from a to R will result in si ðzÞ ¼ Gm

R2 a 2 1 ðwm wm a Þ; a R2 ln Ra 12 ðR2 a2 Þ R

ð24Þ

where m wm R w jr¼R ;

m wm a w jr¼a :

Using Eq. (24) in Eq. (21b) then gives 2 m ðwm R m m R wa Þ srz ¼ G 2 R 1 2 r : R ln a 2 ðR a2 Þ r

ð25a;bÞ

ð26Þ

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1659

Substituting Eq. (26) into Eq. (23b) and integrating with respect to r from a to r will lead to wm ðr; zÞ ¼ wm a þ

R2 ln ar 12 ðr2 a2 Þ m ðw wm a Þ: R2 ln Ra 12 ðR2 a2 Þ R

ð27Þ

To obtain rm zz , it is further assumed that for both the eﬀective ﬁber and the matrix, rrr þ rhh rzz :

ð28Þ

It then follows from Eqs. (4c), (5c) and (28) that rfzz ¼ Ef

owf ; oz

m rm zz ¼ E

owm : oz

ð29a;bÞ

Using Eq. (27) in Eq. (29b) gives m rm zz ¼ ri þ

R2 ln ar 12 ðr2 a2 Þ m ðr j rm i Þ; R2 ln Ra 12 ðR2 a2 Þ zz r¼R

ð30Þ

where m rm i rzz jr¼a

ð31Þ

is the axial normal stress on the interface r = a. To ﬁnd cylinder along the z-direction: Z a Z R rfzz ð2prÞdr þ rm pR2 r ¼ zz ð2prÞdr: 0

rm zz jr¼R ,

consider the force balance of the composite

ð32Þ

a

Using Eqs. (9) and (30) in Eq. (32) and carrying out the algebra will yield h i R2 ln Ra 12 ðR2 a2 Þ m 2 2 f 2 2 m R r a r ðR a Þr rm : zz zz jr¼R ¼ ri þ 4 i 2 2 R 1 R ln a 4 ðR a2 Þð3R a2 Þ

ð33Þ

From Eqs. (10), (24), (29b), (31) and (33) it follows that h i d2 rfzz 1 R2 a 2 1 2 2 f 2 2 m R ¼ r a r ðR a Þr i : zz 1 þ mm a2 R4 ln Ra 14 ðR2 a2 Þð3R2 a2 Þ dz2

ð34Þ

Note that perfect bonding implies that f em zz jr¼a ¼ ezz jr¼a :

ð35Þ

This condition would remain the same if it were to be expressed in terms of the axial normal strain in the nanotube because of the isostrain condition invoked earlier in obtaining Ef from Et (see Eq. (2)). Using Eqs. (4c), (29a,b) and (31) in Eq. (35) then gives Ef m r : ð36Þ Em i Considering that the diameter of the nanotube (and thus of the eﬀective ﬁber) is very small, it is assumed that rfzz ðr; zÞ can be represented, with good accuracy, by its average rfzz ðzÞ. Then, Eq. (36) becomes Em f rm r : ð37Þ i ¼ Ef zz Substituting Eq. (37) into Eq. (34) leads to rfzz jr¼a ¼

d2 rfzz a 2 R2 2 f r; a r ¼ m zz dz2 a2 þ EEf ðR2 a2 Þ

ð38Þ

1660

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

where m

a2 þ EEf ðR2 a2 Þ 1 R2 a2 : a ¼ 1 þ mm a2 R4 ln Ra 14 ðR2 a2 Þð3R2 a2 Þ 2

ð39Þ

The general solution of Eq. (38) is given by rfzz ¼ c1 eaz þ c2 eaz þ

a2

þ

Em Ef

R2 r; ðR2 a2 Þ

where c1 and c2 are two constants to be determined from the boundary conditions. Using Eq. (40) in Eq. (10) yields a si ¼ aðc1 eaz c2 eaz Þ: 2 The substitution of Eqs. (33), (37) and (40) into Eq. (30) leads to h i 8

9 m 2 r 1 2

2

c1 eaz þ c2 eaz þ 2 Em 2 r : a þ Ef ðR a2 Þ Finally, the use of Eq. (41) in Eq. (14b) gives a sfrz ¼ ðc1 eaz c2 eaz Þr; 2 and Eq. (41) in Eq. (21b) results in 2 a2 a R m srz ¼ r ðc1 eaz c2 eaz Þ: 2ðR2 a2 Þ r

ð40Þ

ð41Þ

ð42Þ

ð43Þ

ð44Þ

m Clearly, the interfacial shear stress si and the stress components rfzz ðzÞ, sfrz , rm zz and srz in the eﬀective ﬁber and the matrix in the reinforced region (Lt 6 z 6 Lt) will be completely determined from Eqs. (40)–(44) once the constants c1 and c2 have been found. The determination of c1 and c2 requires the use of the solution in the pure matrix regions.

3.2. Solution in the pure matrix regions (L 6 z 6 Lt and Lt 6 z 6 L) Each of the two pure matrix cylinders at the ends of the RVE may still be viewed as a composite cylinder reinforced by a virtual ﬁber having the same diameter as that of the eﬀective ﬁber (or nanotube) and the same YoungÕs modulus and PoissonÕs ratio as those of the matrix material. As a result, the solution derived above for the composite region (Lt 6 z 6 Lt) can be applied to the pure matrix regions (L 6 z 6 Lt and Lt 6 z 6 L) by replacing Ef with Em. Hence, from Eq. (40) it follows that, with Ef = Em, am z rfm þ c4 eam z þ r; zz ¼ c3 e

ð45Þ

where the superscript fm refers to the virtual ﬁber, c3 and c4 are two unknown constants, and am is obtained from Eq. (39), with Ef = Em, as a2m ¼

1 R2 a 2 R2 : 1 þ mm a2 R4 ln Ra 14 ðR2 a2 Þð3R2 a2 Þ

ð46Þ

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

The use of Eqs. (10) and (45) in Eq. (14b) gives r am z sfm c4 eam z Þ: rz ¼ am ðc3 e 2

1661

ð47Þ

Note that in component form Eq. (6b) reads rm zz jz¼ L ¼ r;

sm rz jz¼ L ¼ 0;

ð48a; bÞ

and Eq. (7b) becomes rfzz jz¼ Lt ;06r6a ¼ rm zz jz¼ Lt ;06r6a ;

sfrz jz¼ Lt ;06r6a ¼ sm rz jz¼ Lt ;06r6a :

ð49a;bÞ

Applying Eq. (48a) to Eq. (45) gives c3 ¼ c4 ¼ 0;

ð50Þ

which leads to, upon its substitution into Eqs. (45) and (47), rfm zz ¼ r;

sfm rz ¼ 0:

ð51a;bÞ

Clearly, Eq. (48b) is satisﬁed by the shear stress component given in Eq. (51b). Next, using Eqs. (40) and (51a) in Eq. (49a) yields " # r R2 1 2 Em 2 c1 ¼ c2 ¼ : 2 coshðaLt Þ a þ Ef ðR a2 Þ

ð52Þ

The substitution of Eq. (52) into Eqs. (40)–(44) will then lead to the stress components in the reinforced region (Lt 6 z 6 Lt). The results give " # ( ) R2 R2 coshðazÞ f þ 1 2 Em 2 rzz ¼ r; ð53aÞ m a2 þ EEf ðR2 a2 Þ a þ Ef ðR a2 Þ coshðaLt Þ 2 2 Em ðR a Þ 1 f aa sinhðazÞ E r; si ¼ m 2 coshðaLt Þ a2 þ EEf ðR2 a2 Þ 2 2 Em ðR a Þ 1 f ra sinhðazÞ E sfrz ¼ r; m 2 coshðaLt Þ a2 þ EEf ðR2 a2 Þ h i 8

9 2 r 1 2

2 2 2 Em 2 < 2 m a þ ðR a Þ R2 ln ar 12 ðr2 a2 Þ = f R ln ðr a Þ R E E a 2 rm rþ zz ¼ 4 : Ef ; R4 ln Ra 14 ðR2 a2 Þð3R2 a2 Þ R ln Ra 14 ðR2 a2 Þð3R2 a2 Þ " # ( ) R2 R2 coshðazÞ

þ 1 2 Em 2 r; m a2 þ EEf ðR2 a2 Þ a þ Ef ðR a2 Þ coshðaLt Þ sm rz

m a2 1 EEf

2 a sinhðazÞ R r r; ¼ m 2 coshðaLt Þ a2 þ EEf ðR2 a2 Þ r

ð53bÞ

ð53cÞ

ð53dÞ

ð53eÞ

where the hollowness of the nanotube is accounted for through Ef (see Eq. (2)). The stress components in the two pure matrix regions can then be readily obtained from Eqs. (53a–e) by letting Ef = Em. The results give

1662

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667 m rfm zz ¼ rzz ¼ r;

m sfm rz ¼ si ¼ srz ¼ 0;

ð54a;bÞ

which represent a homogeneous deformation induced by the uniform uniaxial tension, as expected.

4. Numerical results To illustrate the shear-lag model developed in the preceding section, parametric studies are conducted for nanotube-reinforced polymer composites using the newly derived formulas. Sample numerical results are presented below. Fig. 13 shows how the normalized interfacial shear stress and average axial normal stress in the nanotube vary along the nanotube length for three cases having diﬀerent nanotube aspect ratios (ARs). To compare with the corresponding results of Li and Chou (2003b), values of the controlling parameters for the composite under consideration are taken to be the same as those used in Li and Chou (2003b), i.e., Em = 2.41 GPa, mm = 0.35, Ef = 1000 GPa, a = 0.471 nm, and R = 5a. The ﬁrst two matrix material properties are typical for an epoxy polymer. A comparison shows that in all of the three cases (with diﬀerent aspect ratios) considered the trends of both si/r and rfzz =r varying with z/(2a), as predicted by the current shear-lag model, are the same as those predicted by the computational model of Li and Chou (2003b). Moreover, the magnitudes of both si/r and rfzz =r predicted respectively by the two diﬀerent models are not too far apart, which can be diﬃcult to achieve in continuum-based simulations of nanostructured materials (e.g., Liu and Chen, 2003). These agreements verify the feasibility of the current model. To further demonstrate applications of the new model, a second nanocomposite is considered. At this time the properties of the polymer matrix are taken to be the same as those used above (i.e., Em = 2.41 GPa, mm = 0.35), but the YoungÕs modulus of the eﬀective ﬁber is now Ef = 1006 GPa, which represents the (9, 0) zigzag nanotube with the outer diameter 2a = 0.7086 nm, as listed in Table 1. Again, R = 5a and the same three aspect ratios are used in the current simulation. The results are illustrated in Figs. 14–17.

Fig. 13. Interfacial shear stress (a) and average axial normal stress in the nanotube (b).

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667 2.5 AR=10.1 AR=12.8

2 1.5

AR=7.8

1

τi /σ

0.5 0

-0.5 -1 -1.5 -2 -2.5 -8

-6

-4

-2

0 z/2a

2

4

6

8

Fig. 14. Interfacial shear stress. 2.5 2 r /a = 1

1.5 1

r /a = 2

τ rzm/ σ

0.5

r /a = 5

0 r /a = 3

-0.5

r /a = 4

-1 -1.5 -2 -2.5 -8

-6

-4

-2

0 z/2a

2

4

6

8

Fig. 15. Shear stress in the matrix (with AR = 12.8). 20 18 AR=12.8

16

AR=10.1

14

σ zzf / σ

12

AR=7.8

10 8 6 4 2 0 -8

-6

-4

-2

0 z/2a

2

4

6

Fig. 16. Average axial normal stress in the nanotube.

8

1663

1664

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667 1 0.9 0.8

σ zzm/ σ

0.7 0.6

AR = 7.8

0.5 0.4

AR = 10.1

0.3

AR = 12.8

0.2 -8

-6

-4

-2

0 z/2a

2

4

6

8

Fig. 17. Average axial normal stress in the matrix.

The variation of the interfacial shear stress along the nanotube length is illustrated in Fig. 14, while that of the shear stress in the matrix in Fig. 15. From Fig. 14 it is seen that the maximum shear stress transfer occurs near the two ends of the nanotube, but the middle of the nanotube is shear stress free due to symmetry. Also, the larger the aspect ratio is, the smaller the interfacial shear stress (at the same z and for given a and r) becomes. These agree with those observed in Li and Chou (2003b). Fig. 15 shows that the same is true for the shear stress distribution in the matrix: the maximum of the shear stress occurring at the ends and the minimum (zero-valued) in the center of the reinforcing length (i.e., at z = 0). In addition, it is observed from Fig. 15 that the shear stress sm rz decreases rapidly with the increase of the radial distance from the nanotube–matrix interface and that the traction-free boundary condition on the outer surface of the matrix layer (i.e., r/a = 5 R/a) is exactly satisﬁed, as expected. Fig. 16 shows the distribution of the average axial normal stress in the nanotube along the nanotube length, while Fig. 17 illustrates that of the average axial normal stress in the matrix. Clearly, it is observed from Fig. 16 that the maximum axial normal stress is reached in the middle of the nanotube, whereas the minimum occurs at its two ends. Also, it is seen that the larger the aspect ratio, the higher the average axial normal stress at the same z for given a and r. The opposite trends are seen for the average normal stress in the matrix, as shown in Fig. 17. In fact, this is dictated by the global equilibrium requirement. More importantly, it can be noticed from comparing Figs. 16 and 17 that when the nanotube aspect ratio is sufﬁciently large, most of the applied load in the axial direction can be taken up by the nanotube and the surrounding matrix needs to support only a small portion of the axial loading. For example, when AR = 12.8 the portion of the applied load taken by the nanotube on the cross-section z = 0 is more than three times as large as that by the matrix on the same cross-section, although the cross-sectional area of the matrix is twenty-four times as big as that of the eﬀective ﬁber on z = 0 in the current RVE with R = 5a. However, this is no longer the case if the nanotube aspect ratio becomes small. For instance, when AR = 7.8 both of the nanotube and the matrix on the cross-section z = 0 take about the equal amount of the applied load. These reveal that the nanotube aspect ratio is a critical controlling parameter for nanotube-reinforced composites, and that for signiﬁcant reinforcements nanotubes with large aspect ratios should be used. This observation conforms to what has been found in existing experimental and computational studies (e.g., Qian et al., 2000; Frankland et al., 2003), thereby further supporting the newly developed analytical model.

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1665

5. Summary A shear-lag model for predicting the interfacial stress transfer in carbon nanotube-reinforced polymer composites is developed using a multiscale approach. A concentric composite cylinder embedded with a capped nanotube is utilized as a representative volume element (RVE) to capture the major morphological features of the nanocomposites. The atomistic structure of the capped nanotube is incorporated in the model by using the molecular structural mechanics of Li and Chou (2003a), which leads to the determination of the eﬀective YoungÕs modulus of the nanotube. The capped nanotube is equivalently replaced by an eﬀective (solid) ﬁber having the same diameter and length, whose elastic modulus is determined from that of the nanotube under an isostrain condition. The continuum-based shear-lag analysis is carried out using the elasticity theory for axisymmetric problems, which results in closed-form formulas for calculating the interfacial shear stress and other axial stress components in both the nanotube and the matrix. The formulas are directly applied to sample cases to demonstrate the newly developed model. The numerical results show that the predictions by the current analytical model are in qualitative agreement with those by the computational model of Li and Chou (2003b). The numerical data also reveal that the nanotube aspect ratio plays a critical role in designing the nanotube-reinforced polymer composites, and that the nanotubes with suﬃciently large aspect ratios should be used to achieve better reinforcements. These agree with the ﬁndings from earlier experimental and computational studies. Finally, it should be mentioned that replacing the capped nanotube (discrete) by an eﬀective ﬁber with square ends (continuum) is to make the problem analytically tractable in the context of elasticity. The eﬀect of the caps on YoungÕs modulus of the capped nanotube (Et) is incorporated in Eq. (1) through the parameter b. This eﬀect is subsequently included in the determination of the modulus of the eﬀective ﬁber (Ef) using Eq. (2) and then in the computation of the stress components using Eqs. (53a–e). However, the use of square ends (rather than hemispherical ones) does lead to over-predicted stress concentrations near the two ends of the nanotube, as was also observed by Li and Chou (2003b). This remains to be a major limitation of the new model. Nevertheless, the predicted stress distributions far away from the two tube ends should be fairly accurate, since typical nanotubes tend to have very large aspect ratios and the end eﬀects are localized. In fact, it has been observed in the present study that the eﬀect of capping on the elastic modulus of the nanotube is insigniﬁcant for suﬃciently long and large nanotubes (see Fig. 8). Moreover, the current analysis, as an upper-bound estimate, would lead to conservative designs of nanotube-reinforced polymer composites. Acknowledgments The work reported here is partially funded by a grant from the US AFOSR (Grant # F49620-03-1-0442, with Dr. B.-L. Lee as the Program Manager). This support is gratefully acknowledged. The authors also wish to thank Dr. A.K. Roy of the US AFRL/MLBC for supporting the project. In addition, the authors are indebted to two anonymous reviewers for their helpful comments on an earlier version of this paper. References Ajayan, P.M., Schadler, L.S., Giannaris, C., Rubio, A., 2000. Single-walled carbon nanotube–polymer composites: strength and weakness. Adv. Mater. 12, 750–753. Barber, A.H., Cohen, S.R., Wagner, H.D., 2003. Measurement of carbon nanotube–polymer interfacial strength. Appl. Phys. Lett. 82, 4140–4142. Bower, C., Zhu, W., Jin, S., Zhou, O., 2000. Plasma-induced alignment of carbon nanotubes. Appl. Phys. Lett. 77, 830–832. Chang, T., Gao, H., 2003. Size-dependent elastic properties of a single-walled carbon nanotube via a molecular mechanics model. J. Mech. Phys. Solids 51, 1059–1074.

1666

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

Cooper, C.A., Ravich, D., Lips, D., Mayer, J., Wagner, H.D., 2002. Distribution and alignment of carbon nanotubes and nanoﬁbrils in a polymer matrix. Compos. Sci. Technol. 62, 1105–1112. Cox, H.L., 1952. The elasticity and strength of paper and other ﬁbrous materials. Brit. J. Appl. Phys. 3, 72–79. Frankland, S.J.V., Harik, V.M., 2003. Analysis of carbon nanotube pull-out from a polymer matrix. Surf. Sci. 525, L103–L108. Frankland, S.J.V., Caglar, A., Brenner, D.W., Griebel, M., 2002. Molecular simulation of the inﬂuence of chemical cross-links on the shear strength of carbon nanotube-polymer interfaces. J. Phys. Chem. B 106, 3046–3048. Frankland, S.J.V., Harik, V.M., Odegard, G.M., Brenner, D.W., Gates, T.S., 2003. The stress–strain behavior of polymer–nanotube composites from molecular dynamics simulation. Compos. Sci. Technol. 63, 1655–1661. Fujita, M., Saito, R., Dresselhaus, G., Dresselhaus, M.S., 1992. Formation of general fullerenes by their projection on a honeycomb lattice. Phys. Rev. B 45, 13834–13836. Gao, X.-L., Li, K., 2003. Finite deformation continuum model for single-walled carbon nanotubes. Int. J. Solids Struct. 40, 7329–7337. Glukhova, O.E., Zhbanov, A.I., Torgashov, I.G., Sinitsyn, N.I., Torgashov, G.V., 2003. Ponderomotive forces eﬀect on the ﬁled emission of carbon nanotube ﬁlms. Appl. Surf. Sci. 215, 149–159. Govindjee, S., Sackman, J.L., 1999. On the use of continuum mechanics to estimate the properties of nanotubes. Solid State Commun. 110, 227–230. Haggenmueller, R., Gommans, H.H., Rinzler, A.G., Fischer, J.E., Winey, K.I., 2000. Aligned single-wall carbon nanotubes in composites by melt processing methods. Chem. Phys. Lett. 330, 219–225. Harik, V.M., 2001. Ranges of applicability for the continuum beam model in the mechanics of carbon nanotubes and nanorods. Solid State Commun. 120, 331–335. Harik, V.M., 2002. Mechanics of carbon nanotubes: applicability of the continuum-beam models. Comput. Mater. Sci. 24, 328–342. Harris, P.J.F., 1999. Carbon Nanotubes and Related Structures. Cambridge University Press, Cambridge. Li, C., Chou, T.-W., 2003a. A structural mechanics approach for the analysis of carbon nanotubes. Int. J. Solids Struct. 40, 2487–2499. Li, C., Chou, T.-W., 2003b. Multiscale modeling of carbon nanotube reinforced polymer composites. J. Nanosci. Nanotech. 3, 1–8. Li, K., Gao, X.-L., Roy, A.K., 2003. Micromechanical analysis of three-dimensional open-cell foams using the matrix method for space frame structures. In: Proceedings of the 14th International Conference on Composite Materials (ICCM-14), San Diego, CA, July 14–18, 2003. Liao, K., Li, S., 2001. Interfacial characteristics of a carbon nanotube–polystyrene composite system. Appl. Phys. Lett. 79, 4225–4227. Lilleodden, E.T., Zimmerman, J.A., Foiles, S.M., Nix, W.D., 2003. Atomistic simulations of elastic deformation and dislocation nucleation during nanoindentation. J. Mech. Phys. Solids 51, 901–920. Liu, Y.J., Chen, X.L., 2003. Continuum models of carbon nanotube-based composites using the boundary element method. Electron. J. Bound. Elem. 1, 316–335. Lordi, V., Yao, N., 2000. Molecular mechanics of binding in carbon-nanotube–polymer composites. J. Mater. Res. 15, 2770–2779. Lourie, O., Cox, D.M., Wagner, H.D., 1998. Buckling and collapse of embedded carbon nanotubes. Phys. Rev. Lett. 81, 1638–1641. Maruyama, B., Alam, K., 2002. Carbon nanotubes and nanoﬁbers in composite materials. SAMPE J. 38 (3), 59–68. McCartney, L.N., 1992. Analytical models of stress transfer in unidirectional composites and cross-ply laminates, and their application to the prediction of matrix/transverse cracking. In: Reddy, J.N., Reifsnider, K.L. (Eds.), Local Mechanics Concepts for Composite Material Systems, Proceedings of IUTAM Symposium, Blacksburg, VA, October 28–31, 1991. Springer-Verlag, Berlin, pp. 251– 282. Nairn, J.A., 1997. On the use of shear-lag methods for analysis of stress transfer in unidirectional composites. Mech. Mater. 26, 63–80. Odegard, G.M., Gates, T.S., Nicholson, L.M., Wise, K.E., 2002. Equivalent-continuum modeling of nano-structured materials. Compos. Sci. Technol. 62, 1869–1880. Pantano, A., Parks, D.M., Boyce, M.C., 2004. Mechanics of deformation of single- and multi-wall carbon nanotubes. J. Mech. Phys. Solids 52, 789–821. Popov, V.N., Van Doren, V.E., Balkanski, M., 2000. Elastic properties of single-walled carbon nanotubes. Phys. Rev. B 61, 3078–3084. Qian, D., Dickey, E.C., Andrews, R., Rantell, T., 2000. Load transfer and deformation mechanisms in carbon nanotube–polystyrene composites. Appl. Phys. Lett. 76, 2868–2870. Ru, C.Q., 2000. Eﬀective bending stiﬀness of carbon nanotubes. Phy. Rev. B 62, 9973–9976. Saito, R., Fujita, M., Dresselhaus, G., Dresselhaus, M.S., 1992. Electronic structure of chiral graphene tubules. Appl. Phys. Lett. 60, 2204–2206. Saito, R., Fujita, M., Dresselhaus, G., Dresselhaus, M.S., 1993. Electronic structure and growth mechanism of carbon tubules. Mater. Sci. Eng. B 19, 185–191. Schadler, L.S., Giannaris, S.C., Ajayan, P.M., 1998. Load transfer in carbon nanotube epoxy composites. Appl. Phys. Lett. 73, 3842– 3844. Smith, G.E., Spencer, A.J.M., 1970. Interfacial tractions in a ﬁbre-reinforced elastic composite material. J. Mech. Phys. Solids 18, 81– 100. Thostenson, E.T., Chou, T.-W., 2002. Aligned multi-walled carbon nanotube-reinforced composites: processing and mechanical characterization. J. Phys. D: Appl. Phys. 35, L77–L80.

X.-L. Gao, K. Li / International Journal of Solids and Structures 42 (2005) 1649–1667

1667

Thostenson, E.T., Chou, T.-W., 2003. On the elastic properties of carbon nanotube-based composites: modeling and characterization. J. Phys. D: Appl. Phys. 36, 573–582. Thostenson, E.T., Ren, Z., Chou, T.-W., 2001. Advances in the science and technology of carbon nanotubes and their composites: a review. Compos. Sci. Technol. 61, 1899–1912. Wagner, H.D., 2002. Nanotube–polymer adhesion: a mechanics approach. Chem. Phys. Lett. 361, 57–61. Wagner, H.D., Lourie, O., Feldman, Y., Tenne, R., 1998. Stress-induced fragmentation of multiwall carbon nanotubes in a polymer matrix. Appl. Phys. Lett. 72, 188–190. Wu, Z.J., Ye, J.Q., Cabrera, J.G., 2000. 3D analysis of stress transfer in the micromechanics of ﬁber reinforced composites by using an eigen-function expansion method. J. Mech. Phys. Solids 48, 1037–1063. Yao, N., Lordi, V., 1998. Carbon nanotube caps as springs: molecular dynamics simulations. Phys. Rev. B 58, 12649–12651. Zhang, P., Huang, Y., Geubelle, P.H., Klein, P.A., Hwang, K.C., 2002. The elastic modulus of single-wall carbon nanotubes: a continuum analysis incorporating interatomic potentials. Int. J. Solids Struct. 39, 3893–3906.